#------------------------------------------------------------------------------
#$Date: 2016-02-18 14:25:00 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176728 $
#$URL: svn://www.crystallography.net/cod/cif/8/10/30/8103009.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_8103009
loop_
_publ_author_name
'Shuang Chen'
'Stefan Hoffmann'
'Yurii Prots'
'Jing-Tai Zhao'
'Rüdiger Kniep'
_publ_section_title
;
 Crystal structure of potassium ammonium molybdato phosphate,
 K5-x(NH4)xP[Mo4O14(OH)]2 · 2H2O (x = 2.43)
;
_journal_issue                   1
_journal_name_full
'Zeitschrift für Kristallographie - New Crystal Structures'
_journal_page_first              15
_journal_volume                  224
_journal_year                    2009
_chemical_formula_sum            'H15.72 K2.57 Mo8 N2.43 O32 P'
_chemical_formula_weight         1460.87
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2008-12-9
_audit_creation_method           'WinGX routine-INITIALISE'
_audit_update_record
;
2008-12-11 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   8.4551(6)
_cell_length_b                   22.7312(16)
_cell_length_c                   15.3332(11)
_cell_measurement_reflns_used    2653
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.467
_cell_measurement_theta_min      2.226
_cell_volume                     2947.0(4)
_computing_cell_refinement       'WinCSD (2000)'
_computing_data_collection       'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_molecular_graphics    'Diamond (Crystal Impact, 2004)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measured_fraction_theta_full 0.959
_diffrn_measured_fraction_theta_max 0.959
_diffrn_measurement_device_type  'Rigaku AFC7'
_diffrn_measurement_method       oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.043
_diffrn_reflns_av_sigmaI/netI    0.038
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            9829
_diffrn_reflns_theta_full        30.98
_diffrn_reflns_theta_max         31.00
_diffrn_reflns_theta_min         2.23
_exptl_absorpt_coefficient_mu    3.828
_exptl_absorpt_correction_T_max  0.8666
_exptl_absorpt_correction_T_min  1.0000
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.293
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Platelet
_exptl_crystal_F_000             2754
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.015
_refine_diff_density_max         1.095
_refine_diff_density_min         -1.182
_refine_diff_density_rms         0.201
_refine_ls_goodness_of_fit_ref   1.178
_refine_ls_matrix_type           full
_refine_ls_number_parameters     130
_refine_ls_number_reflns         2476
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.178
_refine_ls_R_factor_all          0.071
_refine_ls_R_factor_gt           0.048
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0448P)²+0.3931P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.095
_refine_ls_wR_factor_ref         0.105
_reflns_number_gt                1988
_reflns_number_total             2476
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            409977.cff
_cod_data_source_block           sc_0240a
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 
;
_cod_original_sg_symbol_H-M      Cmcm
_cod_database_code               8103009
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'x, -y, -z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'-x, y, z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 16 h 0.19662(5) 0.012714(16) 0.14604(2) 0.01628(12) Uani 1 d . . .
Mo2 Mo 16 h 0.18877(5) 0.236403(16) 0.14087(2) 0.01860(13) Uani 1 d . . .
P P 4 c 0.0000 0.12482(8) 0.2500 0.0133(4) Uani 1 d S . .
K1 K 8 f 0.0000 0.13654(9) 0.52455(16) 0.0314(8) Uani 0.659(10) d SP . .
N1 N 8 f 0.0000 0.13654(9) 0.52455(16) 0.0314(8) Uani 0.341(10) d SP . .
K2 K 8 f 0.0000 0.37891(10) 0.0357(2) 0.0319(10) Uani 0.478(10) d SP . .
N2 N 8 f 0.0000 0.37891(10) 0.0357(2) 0.0319(10) Uani 0.522(10) d SP . .
K3 K 4 c 0.0000 0.6165(2) 0.2500 0.047(2) Uani 0.293(16) d SP . .
N3 N 4 c 0.0000 0.6165(2) 0.2500 0.047(2) Uani 0.707(16) d SP . .
O1 O 16 h 0.3272(4) 0.05679(15) 0.0927(2) 0.0276(8) Uani 1 d . . .
O2 O 16 h 0.2902(5) 0.44574(14) 0.0963(2) 0.0299(9) Uani 1 d . . .
O3 O 8 f 0.0000 0.04095(19) 0.1009(3) 0.0191(10) Uani 1 d S . .
O4 O 8 g 0.1869(5) 0.49420(19) 0.2500 0.0190(10) Uani 1 d S . .
O5 O 8 g 0.1491(5) 0.08543(16) 0.2500 0.0156(9) Uani 1 d S . .
O6 O 4 f 0.0000 0.9808(2) 0.2500 0.0181(14) Uani 1 d S . .
O7 O 16 h 0.2892(5) 0.19248(15) 0.0704(2) 0.0312(9) Uani 1 d . . .
O8 O 16 h 0.2776(5) 0.30365(16) 0.1344(2) 0.0344(10) Uani 1 d . . .
O9 O 8 g 0.2693(6) 0.20843(18) 0.2500 0.0188(10) Uani 1 d S . .
O10 O 8 f 0.0000 0.25375(19) 0.0763(3) 0.0237(11) Uani 1 d S . .
O11 O 8 f 0.0000 0.16441(16) 0.1682(3) 0.0157(9) Uani 1 d S . .
O12 O 4 c 0.0000 0.2698(2) 0.2500 0.0182(14) Uani 1 d S . .
OW1 O 4 c 0.0000 0.3915(3) 0.2500 0.054(3) Uani 1 d S . .
OW2 O 4 c 0.0000 0.8645(3) 0.2500 0.036(2) Uani 1 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Mo1 O2 105.63(17) . 15_545 ?
O1 Mo1 O3 101.06(16) . . ?
O2 Mo1 O3 101.26(19) 15_545 . ?
O1 Mo1 O4 101.28(18) . 15_545 ?
O2 Mo1 O4 98.10(17) 15_545 15_545 ?
O3 Mo1 O4 145.11(17) . 15_545 ?
O1 Mo1 O5 91.26(15) . . ?
O2 Mo1 O5 161.70(15) 15_545 . ?
O3 Mo1 O5 81.90(16) . . ?
O4 Mo1 O5 71.16(13) 15_545 . ?
O1 Mo1 O6 160.31(17) . 1_545 ?
O2 Mo1 O6 94.06(17) 15_545 1_545 ?
O3 Mo1 O6 75.03(12) . 1_545 ?
O4 Mo1 O6 74.89(13) 15_545 1_545 ?
O5 Mo1 O6 69.15(14) . 1_545 ?
O1 Mo1 Mo1 118.74(12) . 10_556 ?
O2 Mo1 Mo1 116.50(12) 15_545 10_556 ?
O3 Mo1 Mo1 111.23(12) . 10_556 ?
O4 Mo1 Mo1 33.91(11) 15_545 10_556 ?
O5 Mo1 Mo1 46.90(6) . 10_556 ?
O6 Mo1 Mo1 48.70(3) 1_545 10_556 ?
O1 Mo1 K3 53.31(12) . 5_545 ?
O2 Mo1 K3 133.77(15) 15_545 5_545 ?
O3 Mo1 K3 121.67(14) . 5_545 ?
O4 Mo1 K3 56.43(14) 15_545 5_545 ?
O5 Mo1 K3 52.70(12) . 5_545 ?
O6 Mo1 K3 111.81(7) 1_545 5_545 ?
Mo1 Mo1 K3 65.43(2) 10_556 5_545 ?
O7 Mo2 O8 105.71(19) . . ?
O7 Mo2 O9 100.50(17) . . ?
O8 Mo2 O9 101.10(19) . . ?
O7 Mo2 O10 102.02(18) . . ?
O8 Mo2 O10 98.69(19) . . ?
O9 Mo2 O10 144.57(18) . . ?
O7 Mo2 O11 92.45(15) . . ?
O8 Mo2 O11 160.69(17) . . ?
O9 Mo2 O11 81.51(16) . . ?
O10 Mo2 O11 70.57(14) . . ?
O7 Mo2 O12 161.53(17) . . ?
O8 Mo2 O12 92.75(18) . . ?
O9 Mo2 O12 74.73(13) . . ?
O10 Mo2 O12 75.24(12) . . ?
O11 Mo2 O12 69.30(14) . . ?
O7 Mo2 Mo2 119.97(13) . 11 ?
O8 Mo2 Mo2 116.08(15) . 11 ?
O9 Mo2 Mo2 110.83(14) . 11 ?
O10 Mo2 Mo2 33.75(11) . 11 ?
O11 Mo2 Mo2 46.66(6) . 11 ?
O12 Mo2 Mo2 49.03(4) . 11 ?
O7 Mo2 K1 55.09(13) . 10_556 ?
O8 Mo2 K1 133.55(13) . 10_556 ?
O9 Mo2 K1 122.61(12) . 10_556 ?
O10 Mo2 K1 54.80(14) . 10_556 ?
O11 Mo2 K1 53.44(11) . 10_556 ?
O12 Mo2 K1 111.98(7) . 10_556 ?
Mo2 Mo2 K1 64.892(15) 11 10_556 ?
O7 Mo2 K2 115.11(13) . . ?
O8 Mo2 K2 54.48(15) . . ?
O9 Mo2 K2 140.50(12) . . ?
O10 Mo2 K2 44.44(12) . . ?
O11 Mo2 K2 111.97(7) . . ?
O12 Mo2 K2 76.09(10) . . ?
Mo2 Mo2 K2 66.226(16) 11 . ?
K1 Mo2 K2 92.84(5) 10_556 . ?
O11 P O11 108.6(3) 10_556 . ?
O11 P O5 109.77(10) 10_556 11 ?
O11 P O5 109.77(10) . 11 ?
O11 P O5 109.77(10) 10_556 . ?
O11 P O5 109.77(10) . . ?
O5 P O5 109.2(3) 11 . ?
O2 K1 O2 78.46(16) 16_456 6 ?
O2 K1 O8 120.09(14) 16_456 6 ?
O2 K1 O8 70.85(12) 6 6 ?
O2 K1 O8 70.85(12) 16_456 16_456 ?
O2 K1 O8 120.09(14) 6 16_456 ?
O8 K1 O8 81.94(18) 6 16_456 ?
O2 K1 O3 76.08(11) 16_456 10_556 ?
O2 K1 O3 76.08(11) 6 10_556 ?
O8 K1 O3 138.12(9) 6 10_556 ?
O8 K1 O3 138.12(9) 16_456 10_556 ?
O2 K1 O11 121.59(11) 16_456 10_556 ?
O2 K1 O11 121.59(11) 6 10_556 ?
O8 K1 O11 118.32(10) 6 10_556 ?
O8 K1 O11 118.32(10) 16_456 10_556 ?
O3 K1 O11 60.65(12) 10_556 10_556 ?
O2 K1 O10 140.77(8) 16_456 10_556 ?
O2 K1 O10 140.77(8) 6 10_556 ?
O8 K1 O10 83.31(11) 6 10_556 ?
O8 K1 O10 83.31(11) 16_456 10_556 ?
O3 K1 O10 108.45(14) 10_556 10_556 ?
O11 K1 O10 47.80(11) 10_556 10_556 ?
O2 K1 O7 87.71(10) 16_456 4 ?
O2 K1 O7 162.19(12) 6 4 ?
O8 K1 O7 126.47(12) 6 4 ?
O8 K1 O7 64.28(10) 16_456 4 ?
O3 K1 O7 89.83(10) 10_556 4 ?
O11 K1 O7 57.17(8) 10_556 4 ?
O10 K1 O7 54.02(7) 10_556 4 ?
O2 K1 O7 162.19(12) 16_456 10_556 ?
O2 K1 O7 87.71(10) 6 10_556 ?
O8 K1 O7 64.28(10) 6 10_556 ?
O8 K1 O7 126.47(12) 16_456 10_556 ?
O3 K1 O7 89.83(10) 10_556 10_556 ?
O11 K1 O7 57.17(8) 10_556 10_556 ?
O10 K1 O7 54.02(7) 10_556 10_556 ?
O7 K1 O7 103.32(14) 4 10_556 ?
O2 K1 Mo2 159.49(10) 16_456 10_556 ?
O2 K1 Mo2 113.57(8) 6 10_556 ?
O8 K1 Mo2 80.26(8) 6 10_556 ?
O8 K1 Mo2 112.78(10) 16_456 10_556 ?
O3 K1 Mo2 90.37(10) 10_556 10_556 ?
O11 K1 Mo2 38.17(6) 10_556 10_556 ?
O10 K1 Mo2 30.58(5) 10_556 10_556 ?
O7 K1 Mo2 76.77(8) 4 10_556 ?
O7 K1 Mo2 26.55(7) 10_556 10_556 ?
O2 K1 Mo2 113.57(8) 16_456 4 ?
O2 K1 Mo2 159.49(10) 6 4 ?
O8 K1 Mo2 112.78(10) 6 4 ?
O8 K1 Mo2 80.26(8) 16_456 4 ?
O3 K1 Mo2 90.37(10) 10_556 4 ?
O11 K1 Mo2 38.17(6) 10_556 4 ?
O10 K1 Mo2 30.58(5) 10_556 4 ?
O7 K1 Mo2 26.55(7) 4 4 ?
O7 K1 Mo2 76.77(8) 10_556 4 ?
Mo2 K1 Mo2 50.22(3) 10_556 4 ?
O2 K1 K2 45.50(8) 16_456 6_455 ?
O2 K1 K2 123.96(10) 6 6_455 ?
O8 K1 K2 131.96(11) 6 6_455 ?
O8 K1 K2 50.42(9) 16_456 6_455 ?
O3 K1 K2 87.97(5) 10_556 6_455 ?
O11 K1 K2 93.25(5) 10_556 6_455 ?
O10 K1 K2 95.27(4) 10_556 6_455 ?
O7 K1 K2 43.25(7) 4 6_455 ?
O7 K1 K2 146.47(9) 10_556 6_455 ?
Mo2 K1 K2 119.98(6) 10_556 6_455 ?
Mo2 K1 K2 69.80(4) 4 6_455 ?
O1 K2 O1 61.55(16) 7_455 13 ?
O1 K2 O7 65.65(12) 7_455 7_455 ?
O1 K2 O7 102.40(15) 13 7_455 ?
O1 K2 O7 102.40(15) 7_455 13 ?
O1 K2 O7 65.65(12) 13 13 ?
O7 K2 O7 75.57(17) 7_455 13 ?
O1 K2 O10 130.40(13) 7_455 . ?
O1 K2 O10 130.40(13) 13 . ?
O7 K2 O10 64.75(11) 7_455 . ?
O7 K2 O10 64.75(11) 13 . ?
O1 K2 O2 62.63(10) 7_455 11 ?
O1 K2 O2 111.59(12) 13 11 ?
O7 K2 O2 87.48(10) 7_455 11 ?
O7 K2 O2 161.32(14) 13 11 ?
O10 K2 O2 115.13(10) . 11 ?
O1 K2 O2 111.59(12) 7_455 . ?
O1 K2 O2 62.63(10) 13 . ?
O7 K2 O2 161.32(14) 7_455 . ?
O7 K2 O2 87.48(10) 13 . ?
O10 K2 O2 115.13(10) . . ?
O2 K2 O2 107.98(16) 11 . ?
O1 K2 O8 162.40(13) 7_455 . ?
O1 K2 O8 102.72(10) 13 . ?
O7 K2 O8 113.89(12) 7_455 . ?
O7 K2 O8 61.78(10) 13 . ?
O10 K2 O8 52.45(8) . . ?
O2 K2 O8 134.43(14) 11 . ?
O2 K2 O8 62.69(10) . . ?
O1 K2 O8 102.72(10) 7_455 11 ?
O1 K2 O8 162.40(13) 13 11 ?
O7 K2 O8 61.78(10) 7_455 11 ?
O7 K2 O8 113.89(12) 13 11 ?
O10 K2 O8 52.45(8) . 11 ?
O2 K2 O8 62.69(10) 11 11 ?
O2 K2 O8 134.43(14) . 11 ?
O8 K2 O8 91.50(15) . 11 ?
O1 K2 OW1 129.95(13) 7_455 . ?
O1 K2 OW1 129.95(13) 13 . ?
O7 K2 OW1 127.26(13) 7_455 . ?
O7 K2 OW1 127.26(13) 13 . ?
O10 K2 OW1 82.67(17) . . ?
O2 K2 OW1 69.56(11) 11 . ?
O2 K2 OW1 69.56(11) . . ?
O8 K2 OW1 65.50(12) . . ?
O8 K2 OW1 65.50(12) 11 . ?
O1 K2 Mo2 155.15(11) 7_455 . ?
O1 K2 Mo2 119.66(8) 13 . ?
O7 K2 Mo2 90.97(9) 7_455 . ?
O7 K2 Mo2 61.50(8) 13 . ?
O10 K2 Mo2 27.44(5) . . ?
O2 K2 Mo2 127.75(10) 11 . ?
O2 K2 Mo2 87.71(8) . . ?
O8 K2 Mo2 25.11(7) . . ?
O8 K2 Mo2 70.85(8) 11 . ?
OW1 K2 Mo2 70.45(13) . . ?
O1 K2 Mo2 119.66(8) 7_455 11 ?
O1 K2 Mo2 155.15(11) 13 11 ?
O7 K2 Mo2 61.50(8) 7_455 11 ?
O7 K2 Mo2 90.97(9) 13 11 ?
O10 K2 Mo2 27.44(5) . 11 ?
O2 K2 Mo2 87.71(8) 11 11 ?
O2 K2 Mo2 127.75(10) . 11 ?
O8 K2 Mo2 70.85(8) . 11 ?
O8 K2 Mo2 25.11(7) 11 11 ?
OW1 K2 Mo2 70.45(13) . 11 ?
Mo2 K2 Mo2 47.55(3) . 11 ?
O9 K3 O9 86.0(2) 15 5_455 ?
O9 K3 O5 60.42(11) 15 15 ?
O9 K3 O5 146.4(2) 5_455 15 ?
O9 K3 O5 146.4(2) 15 5_455 ?
O9 K3 O5 60.42(12) 5_455 5_455 ?
O5 K3 O5 153.2(2) 15 5_455 ?
O9 K3 O1 129.47(9) 15 5_455 ?
O9 K3 O1 89.97(9) 5_455 5_455 ?
O5 K3 O1 110.69(12) 15 5_455 ?
O5 K3 O1 56.32(8) 5_455 5_455 ?
O9 K3 O1 89.97(9) 15 8 ?
O9 K3 O1 129.47(9) 5_455 8 ?
O5 K3 O1 56.32(8) 15 8 ?
O5 K3 O1 110.69(12) 5_455 8 ?
O1 K3 O1 128.5(2) 5_455 8 ?
O9 K3 O1 129.47(9) 15 14_456 ?
O9 K3 O1 89.97(9) 5_455 14_456 ?
O5 K3 O1 110.69(12) 15 14_456 ?
O5 K3 O1 56.32(8) 5_455 14_456 ?
O1 K3 O1 100.81(16) 5_455 14_456 ?
O1 K3 O1 55.63(14) 8 14_456 ?
O9 K3 O1 89.97(9) 15 15 ?
O9 K3 O1 129.47(9) 5_455 15 ?
O5 K3 O1 56.32(8) 15 15 ?
O5 K3 O1 110.69(12) 5_455 15 ?
O1 K3 O1 55.63(14) 5_455 15 ?
O1 K3 O1 100.81(16) 8 15 ?
O1 K3 O1 128.5(2) 14_456 15 ?
O9 K3 O4 166.60(17) 15 11 ?
O9 K3 O4 107.45(12) 5_455 11 ?
O5 K3 O4 106.17(18) 15 11 ?
O5 K3 O4 47.02(12) 5_455 11 ?
O1 K3 O4 52.56(9) 5_455 11 ?
O1 K3 O4 81.53(14) 8 11 ?
O1 K3 O4 52.56(9) 14_456 11 ?
O1 K3 O4 81.53(14) 15 11 ?
O9 K3 O4 107.45(12) 15 . ?
O9 K3 O4 166.60(17) 5_455 . ?
O5 K3 O4 47.02(12) 15 . ?
O5 K3 O4 106.17(18) 5_455 . ?
O1 K3 O4 81.53(14) 5_455 . ?
O1 K3 O4 52.56(9) 8 . ?
O1 K3 O4 81.53(14) 14_456 . ?
O1 K3 O4 52.56(9) 15 . ?
O4 K3 O4 59.15(18) 11 . ?
O9 K3 Mo1 155.07(5) 15 5_455 ?
O9 K3 Mo1 89.70(8) 5_455 5_455 ?
O5 K3 Mo1 120.53(15) 15 5_455 ?
O5 K3 Mo1 37.48(6) 5_455 5_455 ?
O1 K3 Mo1 25.84(7) 5_455 5_455 ?
O1 K3 Mo1 111.41(15) 8 5_455 ?
O1 K3 Mo1 74.97(9) 14_456 5_455 ?
O1 K3 Mo1 74.00(10) 15 5_455 ?
O4 K3 Mo1 30.00(5) 11 5_455 ?
O4 K3 Mo1 78.13(12) . 5_455 ?
O9 K3 Mo1 155.07(5) 15 14_456 ?
O9 K3 Mo1 89.70(8) 5_455 14_456 ?
O5 K3 Mo1 120.53(15) 15 14_456 ?
O5 K3 Mo1 37.48(6) 5_455 14_456 ?
O1 K3 Mo1 74.97(9) 5_455 14_456 ?
O1 K3 Mo1 74.00(10) 8 14_456 ?
O1 K3 Mo1 25.84(7) 14_456 14_456 ?
O1 K3 Mo1 111.41(15) 15 14_456 ?
O4 K3 Mo1 30.00(5) 11 14_456 ?
O4 K3 Mo1 78.13(12) . 14_456 ?
Mo1 K3 Mo1 49.13(5) 5_455 14_456 ?
Mo1 O1 K2 165.0(2) . 13 ?
Mo1 O1 K3 100.85(15) . 5_545 ?
K2 O1 K3 94.00(12) 13 5_545 ?
Mo1 O2 K1 136.9(2) 15 6_554 ?
Mo1 O2 K2 129.60(19) 15 . ?
K1 O2 K2 93.22(10) 6_554 . ?
Mo1 O3 Mo1 120.8(2) . 11 ?
Mo1 O3 K1 119.45(11) . 10_556 ?
Mo1 O3 K1 119.45(11) 11 10_556 ?
Mo1 O4 Mo1 112.2(2) 8 15 ?
Mo1 O4 K3 93.57(14) 8 . ?
Mo1 O4 K3 93.57(14) 15 . ?
P O5 Mo1 123.48(16) . . ?
P O5 Mo1 123.48(16) . 10_556 ?
Mo1 O5 Mo1 86.19(13) . 10_556 ?
P O5 K3 131.2(2) . 5_545 ?
Mo1 O5 K3 89.82(15) . 5_545 ?
Mo1 O5 K3 89.82(15) 10_556 5_545 ?
Mo1 O6 Mo1 145.0(2) 10_566 11_565 ?
Mo1 O6 Mo1 87.00(7) 10_566 4_565 ?
Mo1 O6 Mo1 82.60(7) 11_565 4_565 ?
Mo1 O6 Mo1 82.60(7) 10_566 1_565 ?
Mo1 O6 Mo1 87.00(7) 11_565 1_565 ?
Mo1 O6 Mo1 145.0(2) 4_565 1_565 ?
Mo2 O7 K2 172.0(2) . 13 ?
Mo2 O7 K1 98.36(16) . 10_556 ?
K2 O7 K1 89.50(11) 13 10_556 ?
Mo2 O8 K1 138.4(2) . 6_554 ?
Mo2 O8 K2 100.41(19) . . ?
K1 O8 K2 87.14(10) 6_554 . ?
Mo2 O9 Mo2 121.7(2) 10_556 . ?
Mo2 O9 K3 119.05(12) 10_556 5_545 ?
Mo2 O9 K3 119.05(12) . 5_545 ?
Mo2 O10 Mo2 112.5(2) . 11 ?
Mo2 O10 K2 108.13(14) . . ?
Mo2 O10 K2 108.13(14) 11 . ?
Mo2 O10 K1 94.63(14) . 10_556 ?
Mo2 O10 K1 94.63(14) 11 10_556 ?
K2 O10 K1 137.60(17) . 10_556 ?
P O11 Mo2 123.88(15) . 11 ?
P O11 Mo2 123.88(15) . . ?
Mo2 O11 Mo2 86.67(13) 11 . ?
P O11 K1 132.2(2) . 10_556 ?
Mo2 O11 K1 88.39(12) 11 10_556 ?
Mo2 O11 K1 88.39(12) . 10_556 ?
Mo2 O12 Mo2 81.93(7) 11 . ?
Mo2 O12 Mo2 143.6(2) 11 10_556 ?
Mo2 O12 Mo2 86.84(8) . 10_556 ?
Mo2 O12 Mo2 86.84(8) 11 4 ?
Mo2 O12 Mo2 143.6(2) . 4 ?
Mo2 O12 Mo2 81.93(7) 10_556 4 ?
K2 OW1 K2 170.0(3) . 10_556 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O1 1.703(3) . ?
Mo1 O2 1.710(3) 15_545 ?
Mo1 O3 1.914(2) . ?
Mo1 O4 1.923(3) 15_545 ?
Mo1 O5 2.335(3) . ?
Mo1 O6 2.4176(16) 1_545 ?
Mo1 Mo1 3.1912(8) 10_556 ?
Mo1 K3 3.838(3) 5_545 ?
Mo2 O7 1.701(3) . ?
Mo2 O8 1.710(4) . ?
Mo2 O9 1.917(2) . ?
Mo2 O10 1.921(2) . ?
Mo2 O11 2.328(3) . ?
Mo2 O12 2.4368(17) . ?
Mo2 Mo2 3.1953(9) 11 ?
Mo2 K1 3.765(2) 10_556 ?
Mo2 K2 3.963(2) . ?
P O11 1.546(4) 10_556 ?
P O11 1.546(4) . ?
P O5 1.548(4) 11 ?
P O5 1.548(4) . ?
K1 O2 2.808(4) 16_456 ?
K1 O2 2.808(4) 6 ?
K1 O8 2.871(4) 6 ?
K1 O8 2.871(4) 16_456 ?
K1 O3 2.907(5) 10_556 ?
K1 O11 3.025(5) 10_556 ?
K1 O10 3.087(5) 10_556 ?
K1 O7 3.121(4) 4 ?
K1 O7 3.121(4) 10_556 ?
K1 Mo2 3.765(2) 10_556 ?
K1 Mo2 3.765(2) 4 ?
K1 K2 4.2498(4) 6_455 ?
K2 O1 2.857(4) 7_455 ?
K2 O1 2.857(4) 13 ?
K2 O7 2.912(4) 7_455 ?
K2 O7 2.912(4) 13 ?
K2 O10 2.919(5) . ?
K2 O2 3.036(4) 11 ?
K2 O2 3.036(4) . ?
K2 O8 3.280(5) . ?
K2 O8 3.280(5) 11 ?
K2 OW1 3.302(3) . ?
K2 Mo2 3.963(2) 11 ?
K3 O9 2.864(6) 15 ?
K3 O9 2.864(6) 5_455 ?
K3 O5 3.053(5) 15 ?
K3 O5 3.053(5) 5_455 ?
K3 O1 3.134(4) 5_455 ?
K3 O1 3.134(4) 8 ?
K3 O1 3.134(4) 14_456 ?
K3 O1 3.134(4) 15 ?
K3 O4 3.204(6) 11 ?
K3 O4 3.204(6) . ?
K3 Mo1 3.838(3) 5_455 ?
K3 Mo1 3.838(3) 14_456 ?
O1 K2 2.857(4) 13 ?
O1 K3 3.134(4) 5_545 ?
O2 Mo1 1.710(3) 15 ?
O2 K1 2.808(4) 6_554 ?
O3 Mo1 1.914(2) 11 ?
O3 K1 2.907(5) 10_556 ?
O4 Mo1 1.923(3) 8 ?
O4 Mo1 1.923(3) 15 ?
O5 Mo1 2.335(3) 10_556 ?
O5 K3 3.053(5) 5_545 ?
O6 Mo1 2.4176(16) 10_566 ?
O6 Mo1 2.4176(16) 11_565 ?
O6 Mo1 2.4176(16) 4_565 ?
O6 Mo1 2.4176(16) 1_565 ?
O7 K2 2.912(4) 13 ?
O7 K1 3.121(4) 10_556 ?
O8 K1 2.871(4) 6_554 ?
O9 Mo2 1.917(2) 10_556 ?
O9 K3 2.864(6) 5_545 ?
O10 Mo2 1.921(2) 11 ?
O10 K1 3.087(5) 10_556 ?
O11 Mo2 2.328(3) 11 ?
O11 K1 3.025(5) 10_556 ?
O12 Mo2 2.4369(17) 11 ?
O12 Mo2 2.4369(17) 10_556 ?
O12 Mo2 2.4368(17) 4 ?
OW1 K2 3.302(3) 10_556 ?
